G1RTCT D. EXAMPLES F. GUTIÉRREZSOLANA S. CICERO J.A. ALVAREZ R. LACALLE W P 6: TRAINING & EDUCATION


 Denis Austin
 2 years ago
 Views:
Transcription
1 D. EXAMPLES 316
2 WORKED EXAMPLE I Infinite Plate under fatigue Introduction and Objectives Data Analysis 317
3 INTRODUCTION AND OBJECTIVES One structural component of big dimensions is subjected to variable loading conditions everyday: 200 MPa during 12 hours and 20 MPa the rest of the day. During the maximum loading conditions other variable stresses appear, with a variation of 30 MPa (because of vibrations with a frequency 50 Hz). Some NDT are performed, with equipment whose sensitivity is 0.2 mm and no cracks are detected. Considering the component as an infinite plate: a) Determine the crack length which is necessary to crack propagation because of vibrations b) Critical crack length for final failure c) Life time for the component d) Evolution of the crack length with time in order to determine inspection periods 318
4 DATA Material properties: K IC = 100 MPa m 1/2 ΔK th (or ΔK 0 ) = 3 MPa m 1/2 if R = P min /P max = 0.1 ΔK th = 1.5 MPa m 1/2 if R = P min /P max = 0.85 Paris Law: da dn = (ΔK) 2 da/dn in m/cycle when ΔK in MPa m 1/2 319
5 Working conditions are plotted in the next figure: σ ( M P a ) h 2 4 h t ( h ) 320
6 The component geometry can be simplified as: σ 2a 2W The equipment sensitivity is 0.2 mm and no crack has been detected. So, in the worst possible situation 2a = 0.2 mm. 321
7 State I: VIBRATIONS σ ( M P a ) h 2 4 h t ( h ) R = P max /P min = 0.8 ΔK th = 1.5 MPa m 1/2 ΔK = Δσ (π a) 1/2 = 30 (π ) 1/2 = 0.53 MPa m 1/2 < ΔK th Existing cracks don t propagate 322
8 State II: MAIN LOADING CONDITIONS σ ( M P a ) h 2 4 h t ( h ) As R = 0.10 ΔK th = 3.0 MPa m 1/2 ΔK = Δσ (π a) 1/2 = 180 (π ) 1/2 = 3.19 MPa m 1/2 > ΔK th Existing cracks could propagate 323
9 As existing cracks could propagate, it is necessary to determine the crack length for crack propagation because of vibrations: ΔK th = 1.5MPa m 1/2 = 30 π a v a v = 0.80 mm For shorter cracks propagation is only due to main loading variation (Δσ =180 MPa, f = 1/86400 Hz) The critical crack length determined at failure is: K a f I max = σ max = 68 mm π a c = 215 π a f = 100MPa m For crack length over 0.80 mm propagation is due to both main loading variation and vibrations (Δσ = 30 MPa, f = 5 Hz) 1/2 324
10 LIFE TIME: The time necessary to initiate the effects of vibrations to cause crack propagation is determined through the Paris law: 1 a f N = Ln = Ln = 2042 cycles C Y ( Δσ) π a 1 10 (180) π cycles is equivalent to 2042 days or 5.59 years Once this crack length is reached, propagation is due to vibrations (mainly): a 0 = 0.8 mm a f = 68 mm 1 a f 1 68 N = Ln = Ln C Y ( Δσ) π a (30) π cycles is equivalent to 0.73 days 2 = cycles The same day that cracks achive length to propagate due to vibration amplitude, the component fails. SO, LIFE TIME IS 5.59 YEARS. 325
11 The evolution of semicrack length with time is (question d)): a ( m m ) 6 8 It is reasonable to define periodical inspections to check if really cracks propagate over the detectable value of 0.2 mm in total length (i.e. every two years) inspection in 2 years. cracks detected? No 0, 8 0, 1 5,59 ye a r s Yes Evaluate remanent life and take decisions 326
12 WORKED EXAMPLE II Fatigue test Introduction and data Objectives Analysis 327
13 INTRODUCTION AND DATA A fatigue test on a seven wire strand was performed. The maximum applied stress is 0.8 σ u and the amplitude is 390 MPa. The strand is one meter long and the diameter of the wires is 5 mm. The test finished with three broken wires, the central one and two external (which were together), after fatigue cycles (f = 8 Hz). The SEM observation of the failure surfaces gave the following information about crack lengths:  Central wire: 0.25 mm (depth) elliptical crack from non propagated initial defect.  External wire A: 1.32 mm from a non differentiated initial defect.  External wire B: 1.20 mm proceeding from a 0.30 mm in depth initial defect. From a previous tension test, the mechanical behaviour of the strand was obtained: E = 195 GPa Failure Load = kn Strain for Failure Load = 4.7 % (gauge base 500 mm) 328
14 OBJECTIVES From the testing results and the behaviour of the material, determine: a) The failure sequence of the wires as well as their form of failure and the fracture toughness of the material. b) Fatigue behaviour of the material considering a Paris exponent of 2.4 and the depth of the initial defect of wire A. a Consider for the wire geometry that K I = 2.12 σ a
15 The area of each wire is: A w = π r 2 = π = mm 2 Therefore, the area of the strand is A = 7 A w = = mm 2 The failure load is kn, so the failure stress can be calculated: σ f = / =1864 MPa The maximum and minimum stresses are: σ max = 0.8 σ f = = MPa σ min = 0.8 σ f 390 = = MPa 330
16 Under these conditions, the first failure occurs in the external wire A because it has the bigger propagated defect. After that, the external wire B breaks and finally, the central one. The external wire A breaks because of a fracture failure as a consequence of a fatigue process. Then: K I = 2.12 σ a c 0.5 = ( ) 0.5 = MPa m 1/2 K IC = MPa m ½ 331
17 The external wire B also fails because of fracture, but with a smaller defect because the decrease of the section once the external wire A is broken. The new supported σ max is: σ max = 7/ = MPa This stress is smaller than the failure strength of the strand (1864 MPa). Therefore, failure happens as a consequence of sudden fracture or plastic collapse. This later as the applied stress ( MPa) is close to yield stress (even non considering a possible strain hardening effect, then σ ymax = σ u = 1864 MPa) 332
18 We can calculate the stress intensity factor: K I = 2.12 σ a c 0.5 = (0.0012) 0.5 K I = MPa m ½ This value is bigger than K IC and it justifies the sudden failure of the external wire B. Now, there are only five wires in the section of the strand, so: σ max = 6/ = MPa This stress is bigger than the failure stress of the cord (1864 MPa). Therefore, it is possible to affirm that the latest is the maximum stress in the strand, and the central wire fails because of tension. In effect, the necessary stress for fracture to occur would be: = 2.12 σ σ = 3428 MPa Such a value is not reached at any time. 333
19 Let s now determine the fatigue properties of the material. We know that the central wire had a defect of 0.25 mm which did not produce crack propagation under Δσ = 390 MPa. So: ΔK th > 2.12 Δσ a 0.5 = = MPa m 1/2 We also know that an initial defect of 0.3 mm propagates in the external wire B and that the unknown initial defect of wire A should be higher than 0.3 because it reached a bigger final crack. So: ΔK th < 2.12 Δσ a 0.5 = = MPa m 1/2 From both expressions the threshold SIF is limited from the following values: < ΔK th < MPa m 1/2 334
20 The Paris law is: da dn 2.4 = C ( ΔK) = C (2.12 Δσ a ) 2.4 where C has to be defined We know: Δσ = 390 MPa So: da dn = C ( 2.4 ΔK ) = C ( a ) a i a f = da 2. C ( ) 4 dn 1.2 a = a = 0.3 mm C N a i f = 1.2 mm N = cycles conditions at wire B 335
21 C = = Therefore, the Paris law is: da dn = ( ΔK) 2.4 To calculate the initial defect in the external wire A, we will integrate the Paris law: 12 C = a 0.2 i a f = C N a f = 1.32 mm N = cycles a i = C N = a i = mm 336
MAE 20 Winter 2011 Assignment 6
MAE 0 Winter 011 Assignment 6 8.3 If the specific surface energy for sodalime glass is 0.30 J/m, using data contained in Table 1.5, compute the critical stress required for the propagation of a surface
More informationC. PROCEDURE APPLICATION (FITNET)
C. PROCEDURE APPLICATION () 495 INTRODUCTION ASSESSMENT OF SCC ASSESSMENT OF CORROSION FATIGUE STRESS CORROSION AND CORROSION FATIGUE ANALYSIS ASSESSMENT OF LOCAL THINNED AREAS 496 INTRODUCTION INTRODUCTION
More informationFAILURE MODES and MATERIALS PROPERTIES. Component failures. Ductile and Brittle Fracture COMPONENT FAILURES. COMPONENT FAILURE MODES examples:
FAILURE MODES and MATERIALS PROPERTIES MECH2300  Materials Lecture 10 R. W. Truss Materials Engineering R.Truss@uq.edu.au COMPONENT FAILURES Structures lectures es on component es cause response in component
More informationPrinciples of Fracture Mechanics
81 CHAPTER 8 FAILURE PROBLEM SOLUTIONS Principles of Fracture Mechanics 8.1 This problem asks that we compute the magnitude of the maximum stress that exists at the tip of an internal crack. Equation
More informationFatigue Testing. Objectives
Laboratory 8 Fatigue Testing Objectives Students are required to understand principle of fatigue testing as well as practice how to operate the fatigue testing machine in a reverse loading manner. Students
More informationFatigue crack propagation
1 (20) Repetition Ð Crack initiation and growth Small cracks Shear driven Interact with microstructure Mostly analyzed by continuum mechanics approaches Large cracks Tension driven Fairly insensitive to
More informationGriffith theory of brittle fracture:
Griffith theory of brittle fracture: Observed fracture strength is always lower than theoretical cohesive strength. Griffith explained that the discrepancy is due to the inherent defects in brittle materials
More informationME 215 Engineering Materials I
ME 215 Engineering Materials I Chapter 3 Properties in Tension and Compression (Part III) Mechanical Engineering University of Gaziantep Dr. A. Tolga Bozdana www.gantep.edu.tr/~bozdana True Stress and
More information9. TIME DEPENDENT BEHAVIOUR: CYCLIC FATIGUE
9. TIME DEPENDENT BEHAVIOUR: CYCLIC FATIGUE A machine part or structure will, if improperly designed and subjected to a repeated reversal or removal of an applied load, fail at a stress much lower than
More informationσ m using Equation 8.1 given that σ
8. Etimate the theoretical fracture trength of a brittle material if it i known that fracture occur by the propagation of an elliptically haped urface crack of length 0.8 mm and having a tip radiu of curvature
More informationB. INTRODUCTION TO ASSESSMENT PROCEDURES FOR CRACKED COMPONENTS
B. INTRODUCTION TO ASSESSMENT PROCEDURES FOR CRACKED COMPONENTS 40 INTRODUCTION HOW ARE INTEGRITY, SECURITY OR CRITICAL CONDITIONS ANALYSED IN A CRACKED STRUCTURE? FRACTURE MECHANICS Critical conditions
More informationCHAPTER 4 TENSILE TESTING
CHAPTER 4 TENSILE TESTING EXERCISE 28, Page 7 1. What is a tensile test? Make a sketch of a typical load/extension graph for a mild steel specimen to the point of fracture and mark on the sketch the following:
More informationDamage due to fatigue occurs when loading is markedly varying in time. R decreases with time S T. MSÚ F max
5. Fatigue of steel structures Fatigue loading, Wöhler s approach and fracture mechanics, fatigue strength, influence of notches, damage accumulation, Eurocode approach. Damage due to fatigue occurs when
More informationMAE 20 Winter 2011 Assignment 5
MAE 20 Winter 2011 Assignment 5 6.7 For a bronze alloy, the stress at which plastic deformation begins is 275 MPa (40,000 psi), and the modulus of elasticity is 115 GPa (16.7 10 6 psi). (a) What is the
More informationME111 Lecture 16 1. ME111 Instructor: Peter Pinsky Class #16 November 1, 2000
Toda s Topics ME111 Instructor: Peter Pinsk Class #16 November 1, 2000 Introduction to linear elastic fracture mechanics (LEFM). Problem 3 A centercracked plate of AII 1144 steel ( C = 115MPa m ) has
More informationG1RTCT200105071 A. BASIC CONCEPTS F. GUTIÉRREZSOLANA S. CICERO J.A. ALVAREZ R. LACALLE W P 6: TRAINING & EDUCATION
A. BASIC CONCEPTS 472 PROCESSES LOADING RATE Static or QuasiSstatic Dynamic MATERIAL ENVIRONMENT Liquid or Gaseous Environments AGGRESSIVE ENVIRONMENT MECHANIC LOADS Stress corrosion cracking (SCC) Corrosion
More informationSTRAINLIFE (e N) APPROACH
CYCLIC DEFORMATION & STRAINLIFE (e N) APPROACH MONOTONIC TENSION TEST AND STRESSSTRAIN BEHAVIOR STRAINCONTROLLED TEST METHODS CYCLIC DEFORMATION AND STRESSSTRAIN BEHAVIOR STRAINBASED APPROACH TO
More informationCracking Of Carbon Steel Components Due To Repeated Thermal Shock
Cracking Of Carbon Steel Components Due To Repeated Thermal Shock J W H Price, M Chang and B Kerezsi Department of Mechanical Engineering, Monash University, PO Box 197, Caulfield East, VIC 3145, Australia
More informationMechanical Metallurgy
Mechanical Metallurgy Lecturer Assessment Dr. Assignment 20 (homework, quiz, attendance) Midterm exam 40 Final exam 40 Total 100 Mechanical Metallurgy Subject of interests Part I Mechanical fundamentals
More informationCH 6: Fatigue Failure Resulting from Variable Loading
CH 6: Fatigue Failure Resulting from Variable Loading Some machine elements are subjected to static loads and for such elements static failure theories are used to predict failure (yielding or fracture).
More informationME311 Machine Design
ME Machine Design Lecture 5: FullyReversing Fatigue and the SN Diagram W Dornfeld Oct26 Fairfield University School of Engineering Discovering Fatigue With the Industrial Revolution came the steam engine
More informationANALYSIS OF THE FATIGUE STRENGTH UNDER TWO LOAD LEVELS OF A STAINLESS STEEL BASED ON ENERGY DISSIPATION
EPJ Web of Conferences 6, 6 38009 (00) DOI:0.05/epjconf/000638009 Owned by the authors, published by EDP Sciences, 00 ANALYSIS OF THE FATIGUE STRENGTH UNDER TWO LOAD LEVELS OF A STAINLESS STEEL BASED ON
More informationAssessment of Fatigue Cracks in Rails
Procedia  Social and Behavioral Sciences 00 (2011) 000 000 Procedia Social and Behavioral Sciences www.elsevier.com/locate/procedia Conference Title (Transport Research Arena Europe 2012) Assessment of
More informationIMPELLER FATIGUE ASSESSMENT USING AN SN APPROACH
ENGINEERING PAPER 524408 IMPELLER FATIGUE ASSESSMENT USING AN SN APPROACH Samuel Orr Engineering Analysis Manager Howden Technology AMCA International Engineering Conference Las Vegas, NV, USA 2 4 March
More informationObjective To conduct Charpy Vnotch impact test and determine the ductilebrittle transition temperature of steels.
IMPACT TESTING Objective To conduct Charpy Vnotch impact test and determine the ductilebrittle transition temperature of steels. Equipment Coolants Standard Charpy VNotched Test specimens Impact tester
More informationNOTCHES AND THEIR EFFECTS. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 1
NOTCHES AND THEIR EFFECTS Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 1 CHAPTER OUTLINE Background Stress/Strain Concentrations SN Approach for Notched Members
More informationAccelerated Corrosion Fatigue Studies on SA 333 Gr.6 Carbon Steel
Accelerated Corrosion Fatigue Studies on SA 333 Gr.6 Carbon Steel P. S. Aarthi 1, G. Raghava 2, S. Vishnuvardhan 3, M. Surendar 4 P.G. Student, Department of Civil Engineering, Easwari Engineering College,
More information( ) = ( ) = {,,, } β ( ), < 1 ( ) + ( ) = ( ) + ( )
{ } ( ) = ( ) = {,,, } ( ) β ( ), < 1 ( ) + ( ) = ( ) + ( ) max, ( ) [ ( )] + ( ) [ ( )], [ ( )] [ ( )] = =, ( ) = ( ) = 0 ( ) = ( ) ( ) ( ) =, ( ), ( ) =, ( ), ( ). ln ( ) = ln ( ). + 1 ( ) = ( ) Ω[ (
More informationdifferent levels, also called repeated, alternating, or fluctuating stresses.
Fatigue and Dynamic Loading 1 Fti Fatigue fil failure: 2 Static ti conditions : loads are applied gradually, to give sufficient i time for the strain to fully develop. Variable conditions : stresses vary
More informationFatigue Performance Evaluation of Forged Steel versus Ductile Cast Iron Crankshaft: A Comparative Study (EXECUTIVE SUMMARY)
Fatigue Performance Evaluation of Forged Steel versus Ductile Cast Iron Crankshaft: A Comparative Study (EXECUTIVE SUMMARY) Ali Fatemi, Jonathan Williams and Farzin Montazersadgh Professor and Graduate
More informationThe atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C. = 2(sphere volume) = 2 = V C = 4R
3.5 Show that the atomic packing factor for BCC is 0.68. The atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C Since there are two spheres associated
More informationInvestigation of Stress Intensity Factor of Axial Compressor Blade of Helicopter
Investigation of Stress Intensity Factor of Axial Compressor Blade of Helicopter Neelesh V K Mr. Manjunath M V Mr. Devaraj Dept. of Mechanical Engineering Asst prof, Dept. of Mechanical Engineering Asst
More informationREHABILITATION OF THE FIGUEIRA DA FOZ BRIDGE
REHABILITATION OF THE FIGUEIRA DA FOZ BRIDGE A.Rito Proponte, Lda, Lisbon, Portugal J. Appleton A2P Consult, Lda, Lisbon, Portugal ABSTRACT: The Figueira da Foz Bridge includes a 405 m long cable stayed
More informationFlaw Size Acceptance Limits for a Stainless Steel Pressure Vessel
Flaw Size Acceptance Limits for a Stainless Steel Pressure Vessel Consuelo GuzmanLeong Lucius Pitkin, Inc. Richland, Washington, U.S.A. Frederic A. Simonen, Ph.D. Lucius Pitkin, Inc. Richland, Washington,
More informationComparison of typical 3D printing materials [1]
Comparison of typical 3D printing materials [1] ABS Its strength, flexibility, machinability, and higher temperature resistance make it often a preferred plastic for engineers, and professional applications.
More informationDescription of mechanical properties
ArcelorMittal Europe Flat Products Description of mechanical properties Introduction Mechanical properties are governed by the basic concepts of elasticity, plasticity and toughness. Elasticity is the
More informationSolved with COMSOL Multiphysics 4.3
Vibrating String Introduction In the following example you compute the natural frequencies of a pretensioned string using the 2D Truss interface. This is an example of stress stiffening ; in fact the
More informationTensile Testing. Objectives
Laboratory 1 Tensile Testing Objectives Students are required to understand the principle of a uniaxial tensile testing and gain their practices on operating the tensile testing machine. Students are able
More information1. Introduction. 2. Response of Pipelines
1. Introduction Blasting is common in the coal industry to remove rock overburden so that the exposed coal can be mechanically excavated. A portion of the blast energy released is converted to wave energy
More informationPROPERTIES OF MATERIALS
1 PROPERTIES OF MATERIALS 1.1 PROPERTIES OF MATERIALS Different materials possess different properties in varying degree and therefore behave in different ways under given conditions. These properties
More informationMultiaxial Fatigue. Professor Darrell Socie. 20082014 Darrell Socie, All Rights Reserved
Multiaxial Fatigue Professor Darrell Socie 20082014 Darrell Socie, All Rights Reserved Outline Stresses around holes Crack Nucleation Crack Growth MultiaxialFatigue 20082014 Darrell Socie, All Rights
More informationDesign strength of optical glass
Design strength of optical glass Keith B. Doyle Sigmadyne, Inc. Rochester, NY Mark A. Kahan Optical Research Associates Westborough, MA ABSTRACT Brittle materials such as glass do not possess a single
More informationDistinguishing strength from toughness. Understanding fracture toughness.
Lecture notes version 20 Oct 2010 Chapter 8 Fracture and fracture toughness A fractured Liberty Ship 8.1 Introduction and synopsis Distinguishing strength from toughness. Understanding fracture toughness.
More informationValidation of Cable Bolt Support Design in Weak Rock Using SMART Instruments and Phase 2
Validation of Cable Bolt Support Design in Weak Rock Using SMART Instruments and Phase 2 W.F. Bawden, Chair Lassonde Mineral Engineering Program, U. of Toronto, Canada J.D. Tod, Senior Engineer, Mine Design
More informationLecture 14. Chapter 81
Lecture 14 Fatigue & Creep in Engineering Materials (Chapter 8) Chapter 81 Fatigue Fatigue = failure under applied cyclic stress. specimen compression on top bearing bearing motor counter flex coupling
More informationTensile Testing of Steel
C 265 Lab No. 2: Tensile Testing of Steel See web for typical report format including: TITL PAG, ABSTRACT, TABL OF CONTNTS, LIST OF TABL, LIST OF FIGURS 1.0  INTRODUCTION See General Lab Report Format
More informationALLOY 7475 PLATE AND SHEET HIGHEST TOUGHNESS/STRENGTH
ALCOA MILL PRODUCTS ALLOY 7475 PLATE AND SHEET HIGHEST TOUGHNESS/STRENGTH ALLOY 7475 DESCRIPTION Alloy 7475 is a controlled toughness alloy developed by Alcoa for sheet and plate applications that require
More informationPOLITECNICO DI TORINO. Engineering Faculty Master s Degree in Aerospace Engineering. Final Thesis
POLITECNICO DI TORINO Engineering Faculty Master s Degree in Aerospace Engineering Final Thesis DETECTION AND ANALYSIS OF BARELY VISIBLE IMPACT DAMAGE AND ITS PROGRESSION ON A COMPOSITE OVERWRAPPED PRESSURE
More informationProperties of Materials
CHAPTER 1 Properties of Materials INTRODUCTION Materials are the driving force behind the technological revolutions and are the key ingredients for manufacturing. Materials are everywhere around us, and
More informationMETU DEPARTMENT OF METALLURGICAL AND MATERIALS ENGINEERING
METU DEPARTMENT OF METALLURGICAL AND MATERIALS ENGINEERING Met E 206 MATERIALS LABORATORY EXPERIMENT 1 Prof. Dr. Rıza GÜRBÜZ Res. Assist. Gül ÇEVİK (Room: B306) INTRODUCTION TENSION TEST Mechanical testing
More informationMCEN 2024, Spring 2008 The week of Apr 07 HW 9 with Solutions
MCEN 2024, Spring 2008 The week of Apr 07 HW 9 with Solutions The Quiz questions based upon HW9 will open on Thursday, Apr. 11 and close on Wednesday, Apr 17 at 1:30 PM. References to A&J: Chapters 13,
More informationMaster of Simulation Techniques. Lecture No.5. Blanking. Blanking. Fine
Master of Simulation Techniques Lecture No.5 Fine Blanking Prof. Dr.Ing. F. Klocke Structure of the lecture Blanking Sheared surface and force Wear Blanking processes and blanking tools Errors on sheared
More informationMODELING THE EFFECT OF TEMPERATURE AND FREQUENCY ON BITUMENCOATED HELICAL CABLE ELEMENTS
MODELING THE EFFECT OF TEMPERATURE AND FREQUENCY ON BITUMENCOATED HELICAL CABLE ELEMENTS Bjørn Konradsen 1 Technological Analyses Centre, Hybrid Underwater Cables, Nexans Norway Steinar V. Ouren Material
More informationFerrous metal (The sensing distance decreases with nonferrous metal.) Power supply voltage (operating voltage range)
Description The sensors provide excellent results even with difficulttodetect objects, e.g. small or thin parts, wires or bright metals. A variety of types cover a wide range of individual requirements
More informationINFLUENCE OF SHOT PEENING ON CHROMIUM ELECTROPLATED AISI 4340 STEEL FATIGUE STRENGTH
INFLUENCE OF SHOT PEENING ON CHROMIUM ELECTROPLATED AISI 4340 STEEL FATIGUE STRENGTH *Voorwald, H. J. C., Silva, M. P., Costa, M. Y. P., a Pigatin, L. W., Marques, B. M. F. Fatigue and Aeronautic Research
More informationLOADCARRYING CAPACITY OF AXIALLY LOADED RODS GLUEDIN PERPENDICULAR TO THE GRAIN
LOADCARRYING CAPACITY OF AXIALLY LOADED RODS GLUEDIN PERPENDICULAR TO TE GRAIN Prof. Dr.Ing..J. Blaß, Dipl.Ing. B. Laskewitz Universität Karlsruhe (T), Germany Abstract Gluedin rods have been used
More informationFATIGUE PROPERTIES OF 7175 ALUMINIUM ALLOY HAND FORGINGS. Vladivoj Očenášek
1. . 11. 1, Plzeň, Czech Republic, EU FATIGUE PROPERTIES OF 717 ALUMINIUM ALLOY HAND FORGINGS Vladivoj Očenášek SVÚM a.s., Podnikatelská 6, 1 11 Praha 9 Běchovice, Czech Republic, ocenasek@svum.cz Abstract
More informationCHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS
CHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS Concepts of Stress and Strain 6.1 Using mechanics of materials principles (i.e., equations of mechanical equilibrium applied to a freebody diagram),
More informationThe Mechanical Properties of Glass
The Mechanical Properties of Glass Theoretical strength, practical strength, fatigue, flaws, toughness, chemical processes Glass Engineering 150:312 Professor Richard Lehman Department of Ceramics and
More informationFATIGUE ANALYSES OF AERONAUTICAL STRUCTURAL DETAILS OF DIFFERENT COMPLEXITY
FATIGUE ANALYSES OF AERONAUTICAL STRUCTURAL DETAILS OF DIFFERENT COMPLEXITY Paulo M S T de Castro, Paulo F P de Matos, Pedro M G P Moreira, Lucas F M da Silva IDMEC and Faculdade de Engenharia, Universidade
More informationStructural Integrity Analysis
Structural Integrity Analysis 1. STRESS CONCENTRATION Igor Kokcharov 1.1 STRESSES AND CONCENTRATORS 1.1.1 Stress An applied external force F causes inner forces in the carrying structure. Inner forces
More informationInfrared Study of Heat Dissipation under Fatigue Crack Propagation
Infrared Study of Heat Dissipation under Fatigue Crack Propagation O. Plekhov, M. Bannikov, A. erekhina, A. Fedorova Physical foundation of strength Institute of continuous media mechanics RAS str. Ak.
More informationReinforced Concrete Design to BS8110 Structural Design 1 Lesson 5
Lesson 5: Deflection in reinforced concrete beams Content 4.1 Introduction 4. Definitions 4..1 Tension 4.. Compression 4.3 Initial sizing 4.3.1 Worked example 4.4 Reinforcement details 4.5 Anchorage at
More information2. FRACTURE MECHANICS
2. FRACTURE MECHANICS Igor Kokcharov 2.1 DEFECTS Structural materials have inner defects such as cracks, which are extreme stress concentrators. There are technological defects shown in diagrams A and
More informationUniaxial Tension and Compression Testing of Materials. Nikita Khlystov Daniel Lizardo Keisuke Matsushita Jennie Zheng
Uniaxial Tension and Compression Testing of Materials Nikita Khlystov Daniel Lizardo Keisuke Matsushita Jennie Zheng 3.032 Lab Report September 25, 2013 I. Introduction Understanding material mechanics
More informationFATIGUE LIFE OF BOLT SUBJECTED TO FATIGUE LOADING CONDITIONS
20 FATIGUE LIFE OF BOLT SUBJECTED TO FATIGUE LOADING CONDITIONS ABSTRACT K. Din and M. T. H. Ghazali Faculty of Civil Engineering, Universiti Teknologi MARA, Shah Alam, Malaysia Email: kdfila@hotmail.com
More informationOptimum proportions for the design of suspension bridge
Journal of Civil Engineering (IEB), 34 (1) (26) 114 Optimum proportions for the design of suspension bridge Tanvir Manzur and Alamgir Habib Department of Civil Engineering Bangladesh University of Engineering
More informationTime Table. MONDAY (ENSCachan) Session 1 : introduction, linear elastic fracture mechanics Session 2 : Exercises. THURSDAY (ENSCachan)
Time Table MONDAY (ENSCachan) Session 1 : introduction, linear elastic fracture mechanics Session 2 : Exercises TUESDAY (ENSCachan) Session 3 : Numerical Practice. Determination of SIF Session 4 : LEFM
More informationTENSILE TESTING PRACTICAL
TENSILE TESTING PRACTICAL MTK 2B Science Of Materials Ts epo Mputsoe 215024596 Summary Material have different properties all varying form mechanical to chemical properties. Taking special interest in
More informationQuestion 6.5: A steel bar 100 mm (4.0 in.) long and having a square cross section 20 mm
14:440:407 Ch6 Question 6.3: A specimen of aluminum having a rectangular cross section 10 mm 12.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationTensile fracture analysis of blunt notched PMMA specimens by means of the Strain Energy Density
Engineering Solid Mechanics 3 (2015) 3542 Contents lists available at GrowingScience Engineering Solid Mechanics homepage: www.growingscience.com/esm Tensile fracture analysis of blunt notched PMMA specimens
More informationNumerical Analysis of Independent Wire Strand Core (IWSC) Wire Rope
Numerical Analysis of Independent Wire Strand Core (IWSC) Wire Rope Rakesh Sidharthan 1 Gnanavel B K 2 Assistant professor Mechanical, Department Professor, Mechanical Department, Gojan engineering college,
More informationWELD  STATIC AND FATIGUE STRENGTH III
32 WELD  STATIC AND FATIGUE STRENGTH III 1.0 INTRODUCTION A component or a structure, which can withstand a single application of load, may fracture if the same load is applied a large number of times.
More informationFEM analysis of the forming process of automotive suspension springs
FEM analysis of the forming process of automotive suspension springs Berti G. and Monti M. University of Padua, DTG, Stradella San Nicola 3, I36100 Vicenza (Italy) guido.berti@unipd.it, manuel.monti@unipd.it.
More informationMechanical & NonDestructive Testing
Training Objective After watching the program and reviewing this printed material, the viewer will gain an understanding and become familiar with the various methods, equipment, and applications of mechanical
More informationDentistry Fatigue test for endosseous dental implants. Report No.: 1 ASTRA System Ti Design
Dentistry Fatigue test for endosseous dental implants Report No.: 1 ASTRA System Ti Design Client: NT  Trading Time of execution: Mai 2011 Subject of work:   S  24285 Abutment Ti DesignTM  RESULTS
More informationModelling of fatigue crack growth in Inconel 718 under hold time conditions  application to a flight spectrum
Modelling of fatigue crack growth in Inconel 718 under hold time conditions  application to a flight spectrum Erik Lundström, Kjell Simonsson, Tomas Månsson and David Gustafsson Linköping University Post
More informationHip Replacement Failure Analysis and Design Improvement Techniques
Hip Replacement Failure Analysis and Design Improvement Techniques Kevin W. Jansen Ohio Northern University Ada, OH, 45810 Email: kjansen@onu.edu ABSTRACT Hip replacements have been utilized widely to
More informationUltrasonic Technique and Device for Residual Stress Measurement
Ultrasonic Technique and Device for Residual Stress Measurement Y. Kudryavtsev, J. Kleiman Integrity Testing Laboratory Inc. 80 Esna Park Drive, Units 79, Markham, Ontario, L3R 2R7 Canada ykudryavtsev@itlinc.com
More informationEffect of Heat Treatment Process on the Fatigue Behavior of AISI 1060 Steel
International International Journal of ISSI, Journal Vol. of 12 ISSI, (2015), Vol.10 No.1, (2013), pp. 2832 No.1 Effect of Heat Treatment Process on the Fatigue Behavior of AISI 1060 Steel M. Mehdinia
More informationFRETTING FATIGUE UNDER VARYING LOADING BELOW THE FRETTING FATIGUE LIMIT
FRETTING FATIGUE UNDER VARYING LOADING BELOW THE FRETTING FATIGUE LIMIT Yoshiyuki KONDO 1, Chu SAKAE 1, Masanobu KUBOTA 1 and Hiroki KITAHARA 2 1 Kyushu University, Faculty of Engineering, 6101, Hakozaki,
More informationMechanical Properties
Mechanical Properties Elastic deformation Plastic deformation Fracture Plastic Instability and the Ultimate Tensile Strength s u P s s y For a typical ductile metal: I. Elastic deformation II. Stable plastic
More informationCapacitive Proximity Sensor
Capacitive Proximity Sensor X Threaded Cylindrical Capacitive Proximity Sensor Detects almost any kind of metallic and nonmetallic objects, including glass, lumber, water, oil, and plastic. Three choices
More informationMeasuring the Condition of Prestressed Concrete Cylinder Pipe
Measuring the Condition of Prestressed Concrete Cylinder Pipe John Marshall, P.E.I, I J.W. Marshall and Associates, and Paul S. Fisk, President NDT Corporation Introduction Prestressed Concrete Cylinder
More informationPunching shear behavior of steelconcrete composite decks with different shear connectors
Punching shear behavior of steelconcrete composite decks with different shear connectors *XiaoQing Xu 1) and YuQing Liu 2) 1), 2) Department of Bridge Engineering, Tongji University, Shanghai 200092,
More informationNumerical modelling of shear connection between concrete slab and sheeting deck
7th fib International PhD Symposium in Civil Engineering 2008 September 1013, Universität Stuttgart, Germany Numerical modelling of shear connection between concrete slab and sheeting deck Noémi Seres
More informationTENSIONMETER ** code 183_LNRSTW **
Electronic tension meter for applications in textile and wire industry. 9 Tension ranges from 0.1200 cn to 550 dan. Versatile instruments usable for applications in textile industry: e. g. 50 up to max.
More informationFatigue Resistance of High Strength Bolts with Large Diameters
1 Fatigue Resistance of High Strength Bolts with Large Diameters Prof. Peter Schaumann; Dipl.Ing. Frithjof Marten Leibniz Universitaet Hannover Institute for Steel Construction Hannover, Germany schaumann@stahl.unihannover.de;
More informationThe Bending Strength of Pasta
The Bending Strength of Pasta 1.105 Lab #1 Louis L. Bucciarelli 9 September, 2003 Lab Partners: [Name1] [Name2] Data File: Tgroup3.txt On the cover page, include your name, the names of your lab partners,
More informationYield Criteria for Ductile Materials and Fracture Mechanics of Brittle Materials. τ xy 2σ y. σ x 3. τ yz 2σ z 3. ) 2 + ( σ 3. σ 3
Yield Criteria for Ductile Materials and Fracture Mechanics of Brittle Materials Brittle materials are materials that display Hookean behavior (linear relationship between stress and strain) and which
More informationBolting Galvanized Steel
Bolting Galvanized Steel This chapter gives information on the characteristics, advantages and economics of bolted galvanized structures and zinc coated fasteners, and offers comment on bolting procedures
More informationCHARACTERISATION OF A RESONANT BENDING FATIGUE TEST SETUP FOR PIPES
CHARACTERISATION OF A RESONANT BENDING FATIGUE TEST SETUP FOR PIPES J. Claeys 1, J. Van Wittenberghe 2, P. De Baets 2 and W. De Waele 2 2 1 Ghent University, Belgium Ghent University, laboratory Soete,
More informationOperating Temperature Range: 30 to +85ç (Note 1) Operating Humidity Range: 40 to 80%
All non products have been discontinued, or will be discontinued soon. Please check the products status on the Hirose website search at www.hiroseconnectors.com, or contact your Hirose sales representative.
More informationTopology Optimization of Engine Mount Brackets Dr. Dirk Sprengel Ford Werke GmbH
Topology Optimization of Engine Mount Brackets Dr. Dirk Sprengel Ford Werke GmbH Dr. D. Sprengel 6/2007 Topology Optimization of EMS Bracket 1 ( 21 ) EMS Bracket Funktion EMS: Engine Mount System Link
More informationEDEXCEL NATIONAL CERTIFICATE/DIPLOMA MECHANICAL PRINCIPLES OUTCOME 2 ENGINEERING COMPONENTS TUTORIAL 1 STRUCTURAL MEMBERS
ENGINEERING COMPONENTS EDEXCEL NATIONAL CERTIFICATE/DIPLOMA MECHANICAL PRINCIPLES OUTCOME ENGINEERING COMPONENTS TUTORIAL 1 STRUCTURAL MEMBERS Structural members: struts and ties; direct stress and strain,
More informationTutorial: Calculation of paired angular contact bearings
Tutorial: Calculation of paired angular contact bearings A pair of angular contact ball bearings mounted backtoback should be calculated for a load case radial load only, and a second load case tilting
More informationModular Plug Connectors compliant to Cat.6 A Standard
Modular Plug Connectors compliant to Cat.6 A Standard TM3P Series Features. Support HighSpeed LAN transmission Improved performance by two row contact arrangement. Conforms to Cat.6 A requirements of
More informationFRETTING FATIGUE CRACKlNG OF A 936 MW TURBO GENERATOR ROTOR FAILURE ANALYSIS AND REFURBISHMENT
FRETTING FATIGUE CRACKlNG OF A 936 MW TURBO GENERATOR ROTOR FAILURE ANALYSIS AND REFURBISHMENT Dr. K. Schöllhorn 1 Dr. G. Ebi 2 K. Steigleder 1 1 ABB Power Generation Ltd Switzerland 2 SENSOPLAN GmbH
More informationSDNS108 Dynamic response of a reinforced concrete slab leaned on 4 with dimensions subjected to a concentrated loading
Titre : SDNS108  Réponse dynamique d'une dalle en béton a[...] Date : 31/05/2012 Page : 1/9 SDNS108 Dynamic response of a reinforced concrete slab leaned on 4 with dimensions subjected to a concentrated
More informationAnalysis of Slotted Counter Sunk (35NCD16 Steel) Aerospace Fasteners
Analysis of Slotted Counter Sunk (35NCD16 Steel) Aerospace Fasteners A R Abelin Roy Deptt. of ME, Govt. Engineering College, Thrissur, India Christopher Solomon S MMD VSSC, ISRO Thiruvananthapuram, India
More information